Available online at SCIENCE Evaluation of crack initiation angle under mixed mode loading at diverse strain rates


 Emory Webb
 1 years ago
 Views:
Transcription
1 Available online at SCIENCE ELSEVIER Theoretical and Applied Fracture Mechanics 42 (2004) 536 theoretical and applied fracture mechanics Evaluation of crack initiation angle under mixed mode loading at diverse strain rates LH. HernándezGómez *, I. SaucedaMeza, G. UrriolagoitiaCalderón, A.S. Balankin, O. Susarrey Instituto Politécnico Nacional. Sección de Estudios de Posgrado e Investigación de la ESIME, Edificio 5, 3er. Piso de la Unidad Profesional Adolfo López.Mateos, Col. Lindavista México, DF, Mexico Abstraet Crack initiation angle, under mixed mode loading at several strain rates, is analysed using an experimentalnumerical approach. The physical phenomenon for the problem at hand is influenced by the local and global conditions. Qne of such factors is the strain rafe at the crack tipo For this purpose, PMMA plates with centred angled cracks under mixed mode loading were tested. The strain rafe at the neighbourhood of the crack tip before crack propagation was evaluated. Considering that this material is strain rate sensitive, the numerical models were calibrated with the modulus of eiasticity measured in tension tests at the observed strain Tales. Numerical evaluations were performed with the finite eiement method in conjunction with the volume energy density criterion. An improvement in the evaluation of the crack propagation angle was observed. In order to complete the analysis, the crack initiation angle was algo evaluated with the strain energy density factor S, considering the mechanical properties of PMMA, as evaluated at the observed strain rates, and the stress intensity factors k, and k2. Results are in agreement with those observed 2004 Elsevier Ltd. AII rights reserved.. Introduction ing work in []. lt considered the crack initiation Crack propagation stability is an engineering direction for an angled crack which was predicted with the maximum circumferential stress criterion. problem that has attracted attention for many This work inspired the investigation of several years. Much work has been done since the pioneer additional factors that are involved in the fracture process. Crack extension stability was studied. Corresponding author. using the eigenfunction series expansion [2,3]. This address: (LH. Hernández approach wasalso considered in [4] to study the Gómez). influence of transversely applied stress by /$  see front 2004 Elsevier Ltd. Al! rights reserved. doi: 0.06/j.tafmec
2 54 LB. HernándezGómez et al. I Theoretica/ and Applied Fracture Mechanics 42 (2004) 536 including the second term of the series obtained in [2,3]. This was extended for the case oftension and bending [5,6]. Regarding crack path extension, the work in [7] investigated effects caused by the applied load direction,the curvature crack radius and the complete stress and/or energy field. Later, crack growth instability was evaluated numerically [8,9] and experimentally [lo]. All this work is based on the single edge Batch specimen under biaxial loading. Recently, crack initiation and propagation in beams with edge crack under mixed loading was analysed []. This was done by using an energetic approach based on the Stheory [2]. The aforementioned works have shown that there are many factors involved. Some of them are local while others are global. These different factors have to be separated in arder to establish their individual contribution to the fracture process. This complicates further when mixed mode loading conditions are developed. In all these cases, quasistatic loading conditions were assumed. However, when the time of load application varíes, strain rate conditions are developed at the crack tipo In materials, which are rate sensitive, mechanical properties change with the loading rateo In other words, fracture energy decreases with increasing strain rateo This has been observed by others [3,4]. As a consequence, the evaluation of the crack initiation angle must take into account these factors. Under these consideraliaos, the question being: how will the crack initiation angle be affected under mixed mode loading? This situation is analysed in this work following an experimentalnumerical approach. The results are then compared with those obtained by means of the strain energy density factor S [5]. 2. Experimental analysis The experimental work has been divided in two parís. The first part evaluates the PMMA modulus of elasticity at different strain rates and the second part evaluates the crack initiation angle. The objective is to first evaluate the mechanical properlíes under tensile load at the observed strain rates at the crack tip when crack initiation takes place. Table PMMA modulus of elasticityat dilferentstrain Tales Strain rate Ref. (SI) Modulus of elasticity (GPa) [6] [6] This work This work This work [7] [7] This was done with an 8502 Instron machine with several loading rates. Appropriate tension specimens were tested. Table swiunarises this data. For the comparison of this data, it has to be borne in mind, atleast, two points, namely () the compliance of the testing machine and (2) the batch variation characteristics of the raw material. These factors were minimized as much as possible by making direct readings of the specimen deformation on the gage length of the specimen with a strain gage. Resides, all the specimens were produced from the same sheet. For the analysis of crack propagation direction, PMMA plates with central angledcracks were loaded under tension, along its majar axis of symmetry. The crack angle with respect to the horizontal plane was set to be 0, 30, 45 and 60. Fig. shows the dimensions of the specimens. In all these cases, the strain field was evaluated with a strain gage located at the crack tip neighbourhood. Specimens were tested with a 8502 Instron machifle with the following loading rates: 300 and 3000mm!min and the strain field variation was recorded with a SYSTEM O0 of Vishay of Measurement Group, Inc. Reproducibility of the results was checked, by testing 0 specimens with the same geometrical conditions. It is important to keep in mind that, it is difficult to establish the strain rate at the very crack tiposo, an average evaluation was obtained with a 3mm strain gage located as clase as possible to the very crack tipo The case of 0 is well known and the results were used to validate the experimental and numerical results. A typical strain rate history is shown in Fig. 2. This corresponds to a specimen tested at 3000mm/min with an horizontal crack. As it can
3 L.H. HernándezGómez et al I Theoreticaland Applied Fracture Mechanics 42 (2004) 536/ 55 I~ 50mm.,~ 50mm. 5mm ~ ~p 8~ 28mm. 5~mm I~ ~ 8mm I.:! mm 28mm (a) (b) I~ 50mm. I~ 50mm., :Jp 8m~~ 8mm 28mm jp 8 mmjj~ ~~mm 28 min (e) (d) Fig.l. Dimension ofthe cracked specimens and strain gage location.ln al! cases the thickness is 6.35mm. (a) 0, (b) 30, (c) 45 and (d) 60. be seen, the strain cate varies as the loading process takes place. Crack initiation is well defined with a curve peak. 3. Numerical analysis The numerical work has been divided in three parts: () Model development, (2) Model calibration and (3) Evaluation of crack initiation direction.more specifically,franc code [8] was used for this purpose. A finite element model with 4300 nodes was generated. This mesh has rectangular elements of eight nodes and eight quarter point elements were used at the crack tipo The whole plate was simulated because there no sym metry prevails when angled cracks are introduced. Crack initiation angle was evaluated with the energy density criterion. In this case, K and Ku are required for these calculations. In order to validate FRANC for this purpose, these parameters were evaluated under quasistatic loading with the same geometry of the cracked specimens. They were loaded quasistatically.. in the same range. The numerical results were compared with those obtained with photoelasticity, using polycarbonate specimens. Convergence between the experimental and numerical results was obtained. This suggests that FRANC is adequate for such calculations. In a second step, the model calibration was done. Its purpose was to obtain the numerical reproduction of the strain cate recorded by the
4 56 LB. HernándezGómez et al. I Theoretica/ and Applied Fracture Mechanics 42 (2004) 53fi E e E Cñ o TIme (sec.) Fig. 2. Strain rate at the crack tip neighbourhood of a specimen with an horizontal crack, and tested with a loading rate of 3000mm/min. strain gages bonded near the crack tipo All the calculations were performed with the same loading rate that was applied by the testing machine. Besides, in order to make a comparison, another finite element analysis was done with the typical modulus of easticity under quasistatic loading (2.9GPa) commonlyreported in the open literature, as in [6]. In Fig. 3, it is shown the typical divergence between these results. This situation was improved when the value of the modulus of elasticity at the observed strain rate, during the loading process, was introduced in the calculations. As shown in Fig. 4, both results are in agreement. In the third step, the fracture analysis of the centred angled crack plate, loaded under tension, '\ E e "(ij Cñ Experimental .Numerical o. Time (sec.) 0. Fig. 3. Divergence between the numerical evaluation of the strain rate under quasistatic conditions and the experimental resu!ts.
5 LH. HernándezGÓmez et al. I Theoretícaland Applied Fracture Medlanícs 42 (2004) 536/ E E ; éi Experimental Numerical O (a) Time (sec) E 0.00 Ē c: 'ro éi Experimental Numerical (b) O Time (sec) Fig.4. Converge between numerical and experimental evaluation of the strain rafe at the crack tip neighbourhood, (a) 300mm/min, (b) 3000mm/min. was done. KI and Kn were evaluated. In arder to make a comparison, this evaluation was made with the mechanical properties at the observed strain rates and under quasistatic loading. In the last case, a modulus of elasticity, equals to 2.9GPa was also taken into account. Crack initiation angle was evaluated in accordance with the energy criterían with the following equation: 2KIKII () = arc tan 2 2 [ KI + KII] The results are summarised in Table 2. () 4. Analysis with the strain energy density concept Another way to evaluate the crack initiation angle is with the fracture theory based on the field strength of the local strain energy density pro po sed in [5]. In this case, the energy release rate is not required and mixed moje crack extension problems may be treated. The fundamental parameter of this theory, the strain energy density factor S, is direction sensitive and it is evaluated in two dimensions with the following relation:
6 58 LB. HernándezGómez et al. I Tlzeoretical and Applied Fracture Meclzanics 42 (2004) 53~ Table 2 Crack initiation angle evaluated with the energy criterion under quasistatic and dynamic loading Crack Load speed K quasistatic K observed KII quasistatic KII observed Crack Crack initiation angle (O) (mm/min) (MpamI/2) strain raje (MPamI/2) strain raje initiation angle angle at observed (MPamI/2) (MpamI/2) quasistatic (O) strain rate (O) O O s = al!~ + 2al2kk2+ a22~ (2) where k and k2 are the stress intensity factors under loading mode I and, respectively. These parameters are related to the energy release rafe, in generalized plane stress, there results G= (nk )/E and Gil = (n~)/e. The coefficients aij (i,j =,2) are given by al! = l6jl [(34v  cos 0)( + cos O)] a2 = ~Jl2 sin O[cos O (  2v)] a22 = l6jl[4( v)(l  coso) + ( + cos 0)(3cos O)] (3) where Ois the polar angle, which varies around the crack tip, v is the Poisson's ratio and Jlis the shear modulus of elasticity. Fig. 5 shows the parameters involved in the crack initiation angle evaluation at the crack tip neighbourhood. Once S is established, crack initiation will take place in a radial direction O, from the crack tip, along which the strain energy density is minimum. Hence the crack initiation angle determined from as =0 00 (4) In this work, the crack inciination angle is taken into account in the calculations by means of the values of the SIF k and kz, because their values are function of the orientation of the crack planeo These parameters were caiculated numerically with the finite element method. Besides, the shear mody Fig. 5. Parameters involved in the calculation of the crack initiation angle. ulus is strain rafe dependent, therefore it was calculated from the modulus of elasticity observed during the experimental tests. The results obtained are shown in Table 3 and they are comparedwith those obtained with the maximum circumferential stress criterion. In all the cases reported in Table 3, the load speed was 3000rnm/min. These are the situations, which are more sensitive to the strain rafe. 5. Discussion of the results The tension tests have shown that PMMA becomes more rigid as the strain rafe increases. This is reflected with the increment of the modulus of elasticity as the strain rafe growths. Comparing KI and Kn evaluations at the observed strain rates ay ay 'Ixy ax x
7 Table 3 L.H. HernándezGómez et al. / Theoretical and Applied Fracture Mechanics 42 (2004) 53ól 59 Crack initiation angle evaluated with the strain energy density factor S and the rnaxirnurn circurnferential stress criterion Crack inclination angle Crack initiation angle This work Strain energy density concept Maxirnurn circurnferential stress with those made under quasistatic conditions (Table 2) a divergence of results is found. In fact, the biggest difference of K values is for angles lesser than 45. This is the range in which K is a dominant factor in the fracture process. On the other hand, the upper divergence of Kn líes on the range of angles greater than 45. This is the case in which this parameter plays an important role in crack direction. In the case of the specimen with an horizontal crack, Kn should be zero. Nonetheless, the numerical results show that this value is small. This can be explained by the fact that the whole plate was modelled and some nades may not lay on the crack plane, especially with those that are used in the fracture parameters calculation. Regarding the crack initiation angle, it is neariy O. This was expected. In spite of these differences, it can be considered that the numerical evaluations are in line with reality. With respect to the other cases, the specimens have been made in such a way that the crack runs along the horizontal plane, because Fig. 6. Fracture surface of a 60 cracked specirnen tested at 3rnrn/rnin.
8 60 LH. HernándezGómez et al. I Theoretical ami App/ied Fracture Mechanics 42 (2004) 53{j Fig. 7. Fracture surface of a 60 cracked specimen tested at 3000mm/min. it is perpendicular to the applied tension loado This situation is observed when all the calculations are made with the parameters obtained with the calibrated mojel at the observed strain rateo When quasistatic conditions are applied it can be seen there is some divergence. The crack surfaces were microscopically analysed. Typical results are shown in Figs. 6 and 7, in which the real image is magnified 35 times. In both cases, the initial crack front is on the top of each picture. This is the limit between the mark left by tool that completed the crack front, and the crack surface. In the last afea, different sofí of marks are depicted. In the case of the specimen tested at low strain rate (Fig. 6), the crack surface clase to the crack front has many ribs. On the other hand, the crack loaded with the biggest strain rate (Fig. 7), has a surface which is "clean". This reflects that the latter has used less energy. As the crack propagates, there is a bright regían and at a far distance from the crack front the surface becomes rough. Nonetheless, in the case where a lower strain rate was applied (Fig. 6), there are deeper marks. In other words, as the strain rate increases, the crack surface is smoother. It is important to mentían that this evaluation reflects the fact that less fracture energy is required as the strain rate increases. To complete the discussion, the results with the highest strain rate were compared with those obtained with the strain energy density factor S and the maximum circurnferential stress. As it can be seen, the results of this work and those obtained with the S factor are in agreement. Besides, the case of the horizontal crack (0 ), the crack initiation angle is 0, as it was expected. In accordance with the author's opinion, two points have to be kept in mind when this approach is followed. Namely, () the material mechanical properties at the observed strain rates are easily introduced in the calculations by means of the coefficients all, a2 and a22and (2) the SIF's have to be evaluated as accurate as possible. These should lead to an exact evaluation of the crack angle initiation under
9 L.H. HernándezGómez et al. I Theoretical and Applied Fracture Mechanics 42 (2004) mixed loading mode, as the material is strain rafe dependent. Finally, the work in [5]has shown that the predictions based on the maximum stress criterion do deviate from those obtained by the strain energy density criterion. The results reported in Table 3 are in agreement with ibis statement. 6. Concusions The accurate evaluation. of the stress intensity factors of a crack under mixed mode loading is relevant in arder to establish the crack initiation angle. However, when the strain rafe increases at the crack tip, a quasistatic evaluation may no be valido Under ibis scheme, the crack direction angle of propagation calculated varíes in relation with the one observed in quasistatic conditions. This is confirmed with the values of fracture parameters, such as K and KIl' The calculations are improved when the changes of mechanical properties with strain rafe are taken into account. This situation is also valid when the strain energy density factor S is applied. The crack initiation angle was calculated along the radial direction on which the strain energy density is a mínimum. The obtained results are in agreement with those observed experimentally. AIso, ibis confirms the fact that the stationary value of Smin can be used as an intrinsic material parameter, and from ibis a mixed mode fracture criterion can be stated. Resides, the expected divergence with maximum circumferential stress was also observed. Acknowledgments The grant U awarded by Consejo Nacional de Ciencia y Tecnología and the support given to ibis project by COF AA and CGEPI of Instituto Politécnico Nacional are gratefui acknowledged. AIso, the authors thank Mr. Cándido Zamora for the final numerical cal  culations. References [] F. Erdogan, O.e. Sih, On crack extension in plates under plane loading and transverse shear, J. Basic Eng. Trans. ASME 85(D) (963) [2] B. Cotterell, On brittle fracture paths, In!. J. Fract. Mech. (965) [3] B. Cotterell, Notes on the paths and stability of cracks, Int. J. Fract. TechnoI. 2 (966) [4] J.O. Williams, P.D. Ewing, Fracture under complex stress: The angled crack problem, Int. J. Frac!. Mech. 8 (972) [5] L Finnie, A. Saith, A note on the angled crack problem and directional stability of a crack, In!. J. Frac!. 9 (973) [6] P.D. Ewing, J.L Swedlow, Further results on the angled crack problem, In!. J. Fract. 2 (976) [7] M.E. Kipp, O.C. Sih, The strain energy density failure criterion applied to notched elastic solids, Int. J. Solids Struc!. (975) [8] O. UrriolagoitiaCalderón, LH. HernándezOómez, Evaluation of crack propagation stability with the Williams stress function. Part, Int. J. Compu!. Struct. 6 (4) (996) [9] O. UrriolagoitiaCalderón, L.H. HernándezOómez, Evaluation of crack propagation stability with the Williams stress function. Part II, Int. J. Computo Struct. 63 (5) (997) [0] O. UrriolagoitiaCalderón, LH. Hernández Oómez, Experimental analysis of crack propagation stability in single edge notch specimens, Theor. AppI. Fract. Mech. 28 (997) [] L Nobile, Mixed mode crack initiation and direction in beams with edge crack, Theor. AppI. Fract. Mech. 33 (2000) [2] O.C. Sih, Strain density factor applied to mixed mode crack problems, Int. J. Frac!. 0 (974) [3] O.C. Sih, D.Y. Tzou, Dynamic fracture tale of Charpy V notch specimen, Theor. AppI. Fract. Mech. 5 (986) [4] L.H. HernándezOómez, C. Ruiz, Assessment of data for dynamic crack initiation under shock pressure loading: Part IExperiment, Theor. AppI. Fract. Mech. 9 (993) [5] O.C. Sih, Mechanics of Fracture Initiation and Propagation, Kluwer Academic Publishers, Dordrecht, 99, pp [6] LCJ. The properties of "Pespex" acrylic materials, Plastics Division, Welwyn. [7] LH. HernándezOómez, C. Ruiz, Assessment of data for dypamic crack initiation under shock pressure loading: Part IIAnalysis, Theor. AppI. Fract. Mech. 9 (993) [8] D. Swenson, J. Mark, FRANC2D/L: A crack propagation simulator for plane layered structures, version.3 User's guide, Kansas State University.
Tensile fracture analysis of blunt notched PMMA specimens by means of the Strain Energy Density
Engineering Solid Mechanics 3 (2015) 3542 Contents lists available at GrowingScience Engineering Solid Mechanics homepage: www.growingscience.com/esm Tensile fracture analysis of blunt notched PMMA specimens
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationEstimation of the crack propagation direction in a mixedmode geometry via multiparameter fracture criteria
Focussed on characterization of crack tip fields Estimation of the crack propagation direction in a mixedmode geometry via multiparameter fracture criteria L. Malíková, V. Veselý Brno University of Technology,
More informationNOTCHES AND THEIR EFFECTS. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1
NOTCHES AND THEIR EFFECTS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations SN Approach for Notched Members
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationCOMPUTATIONAL ENGINEERING OF FINITE ELEMENT MODELLING FOR AUTOMOTIVE APPLICATION USING ABAQUS
International Journal of Advanced Research in Engineering and Technology (IJARET) Volume 7, Issue 2, MarchApril 2016, pp. 30 52, Article ID: IJARET_07_02_004 Available online at http://www.iaeme.com/ijaret/issues.asp?jtype=ijaret&vtype=7&itype=2
More informationANALYTICAL AND EXPERIMENTAL EVALUATION OF SPRING BACK EFFECTS IN A TYPICAL COLD ROLLED SHEET
International Journal of Mechanical Engineering and Technology (IJMET) Volume 7, Issue 1, JanFeb 2016, pp. 119130, Article ID: IJMET_07_01_013 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=7&itype=1
More informationNumerical modelling of shear connection between concrete slab and sheeting deck
7th fib International PhD Symposium in Civil Engineering 2008 September 1013, Universität Stuttgart, Germany Numerical modelling of shear connection between concrete slab and sheeting deck Noémi Seres
More informationBending, Forming and Flexing Printed Circuits
Bending, Forming and Flexing Printed Circuits John Coonrod Rogers Corporation Introduction: In the printed circuit board industry there are generally two main types of circuit boards; there are rigid printed
More informationLOADCARRYING CAPACITY OF AXIALLY LOADED RODS GLUEDIN PERPENDICULAR TO THE GRAIN
LOADCARRYING CAPACITY OF AXIALLY LOADED RODS GLUEDIN PERPENDICULAR TO TE GRAIN Prof. Dr.Ing..J. Blaß, Dipl.Ing. B. Laskewitz Universität Karlsruhe (T), Germany Abstract Gluedin rods have been used
More informationTechnology of EHIS (stamping) applied to the automotive parts production
Laboratory of Applied Mathematics and Mechanics Technology of EHIS (stamping) applied to the automotive parts production Churilova Maria, SaintPetersburg State Polytechnical University Department of Applied
More informationMultiaxial Fatigue. Professor Darrell Socie. 20082014 Darrell Socie, All Rights Reserved
Multiaxial Fatigue Professor Darrell Socie 20082014 Darrell Socie, All Rights Reserved Outline Stresses around holes Crack Nucleation Crack Growth MultiaxialFatigue 20082014 Darrell Socie, All Rights
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationSTRESSINTENSITY FACTORS BY BOUNDARY COLLOCATION FOR SINGLEEDGENOTCH SPECIMENS SUBJECT TO SPLITTING FORCES. by Bernard Gross and John E.
NASA TECHNICAL NOTE TN D3295.. STRESSINTENSITY FACTORS BY BOUNDARY COLLOCATION FOR SINGLEEDGENOTCH SPECIMENS SUBJECT TO SPLITTING FORCES by Bernard Gross and John E. SrawZey Lewis Research Center
More informationShort and Large Crack, MixedMode FatigueCrack Growth Thresholds in Ti6Al4V 1
Short and Large Crack, MixedMode FatigueCrack Growth Thresholds in Ti6Al4V 1 Mr. R. K. Nalla, Dr. J. P. Campbell and Professor R. O. Ritchie 2 Department of Materials Science and Engineering University
More informationELASTOPLASTIC ANALYSIS OF A HEAVY DUTY PRESS USING F.E.M AND NEUBER S APPROXIMATION METHODS
International Journal of Mechanical Engineering and Technology (IJMET) Volume 6, Issue 11, Nov 2015, pp. 5056, Article ID: IJMET_06_11_006 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=6&itype=11
More informationDESIGN OF SLABS. 3) Based on support or boundary condition: Simply supported, Cantilever slab,
DESIGN OF SLABS Dr. G. P. Chandradhara Professor of Civil Engineering S. J. College of Engineering Mysore 1. GENERAL A slab is a flat two dimensional planar structural element having thickness small compared
More informationTorsion Testing. Objectives
Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials
More informationMeasurement of Residual Stress in Plastics
Measurement of Residual Stress in Plastics An evaluation has been made of the effectiveness of the chemical probe and hole drilling techniques to measure the residual stresses present in thermoplastic
More informationME111 Lecture 16 1. ME111 Instructor: Peter Pinsky Class #16 November 1, 2000
Toda s Topics ME111 Instructor: Peter Pinsk Class #16 November 1, 2000 Introduction to linear elastic fracture mechanics (LEFM). Problem 3 A centercracked plate of AII 1144 steel ( C = 115MPa m ) has
More informationEFFECTS OF SHOTPEENING ON HIGH CYCLE FRETTING FATIGUE BEHAVIOR OF Ti6Al4V
JOURNAL OF AERONAUTICS AND SPACE TECHNOLOGIES JANUARY 2003 VOLUME 1 NUMBER 1 (5164) EFFECTS OF SHOTPEENING ON HIGH CYCLE FRETTING FATIGUE BEHAVIOR OF Ti6Al4V Halil Ibrahim Air Services Schools and
More informationObjective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels.
IMPACT TESTING Objective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels. Equipment Coolants Standard Charpy VNotched Test specimens Impact tester
More informationPunching shear behavior of steelconcrete composite decks with different shear connectors
Punching shear behavior of steelconcrete composite decks with different shear connectors *XiaoQing Xu 1) and YuQing Liu 2) 1), 2) Department of Bridge Engineering, Tongji University, Shanghai 200092,
More informationMATERIALS AND SCIENCE IN SPORTS. Edited by: EH. (Sam) Froes and S.J. Haake. Dynamics
MATERIALS AND SCIENCE IN SPORTS Edited by: EH. (Sam) Froes and S.J. Haake Dynamics Analysis of the Characteristics of Fishing Rods Based on the LargeDeformation Theory Atsumi Ohtsuki, Prof, Ph.D. Pgs.
More informationMASTER DEGREE PROJECT
MASTER DEGREE PROJECT Finite Element Analysis of a Washing Machine Cylinder Thesis in Applied Mechanics one year Master Degree Program Performed : Spring term, 2010 Level Author Supervisor s Examiner :
More informationCH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More informationEXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR PRODUCTION ON THE PIERCED FLAT SHEET METAL USING LASER FORMING PROCESS
JOURNAL OF CURRENT RESEARCH IN SCIENCE (ISSN 23225009) CODEN (USA): JCRSDJ 2014, Vol. 2, No. 2, pp:277284 Available at www.jcrs010.com ORIGINAL ARTICLE EXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR
More informationStress Strain Relationships
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
More informationSheet metal operations  Bending and related processes
Sheet metal operations  Bending and related processes R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Table of Contents 1.QuizKey... Error! Bookmark not defined. 1.Bending
More informationUse of Strain Gauge Rosette to Investigate Stress concentration in Isotropic and Orthotropic Plate with Circular Hole
Use of Strain Gauge Rosette to Investigate Stress concentration in Isotropic and Orthotropic Plate with Circular Hole Mr.V.G.Aradhye 1, Prof.S.S.Kulkarni 2 1 PG Scholar, Mechanical department, SKN Sinhgad
More informationComposite structures are used extensively in aircraft, space vehicles, marine, and automotive
Finite Element Analyses of CompositetoSteel Adhesive Joints YuPing Yang George W. Ritter David R. Speth Edision Welding Institute Columbus, Ohio Finite element modeling can assist in the design of an
More informationScienceDirect. The Numerical Analysis of the Joint of the Steel Beam to the Timber Girder
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 91 (2014 ) 160 164 XXIII RSP seminar, Theoretical Foundation of Civil Engineering (23RSP) (TFoCE 2014) The Numerical Analysis
More informationSTATIC AND DYNAMIC ANALYSIS OF CENTER CRACKED FINITE PLATE SUBJECTED TO UNIFORM TENSILE STRESS USING FINITE ELEMENT METHOD
INTERNATIONAL JOURNAL OF MECHANICAL ENGINEERING AND TECHNOLOGY (IJMET) International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 6340(Print), ISSN 0976 6340 (Print) ISSN 0976 6359
More informationResearch on the fracture behavior of PBX under static tension
Available online at www.sciencedirect.com ScienceDirect Defence Technology 10 (2014) 154e160 www.elsevier.com/locate/dt Research on the fracture behavior of PBX under static tension Hu GUO*, Jingrun LUO,
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationAnalysis of Stresses and Strains
Chapter 7 Analysis of Stresses and Strains 7.1 Introduction axial load = P / A torsional load in circular shaft = T / I p bending moment and shear force in beam = M y / I = V Q / I b in this chapter, we
More informationThe Bending Strength of Pasta
The Bending Strength of Pasta 1.105 Lab #1 Louis L. Bucciarelli 9 September, 2003 Lab Partners: [Name1] [Name2] Data File: Tgroup3.txt On the cover page, include your name, the names of your lab partners,
More informationBack to Elements  Tetrahedra vs. Hexahedra
Back to Elements  Tetrahedra vs. Hexahedra Erke Wang, Thomas Nelson, Rainer Rauch CADFEM GmbH, Munich, Germany Abstract This paper presents some analytical results and some test results for different
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More informationYield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials. τ xy 2σ y. σ x 3. τ yz 2σ z 3. ) 2 + ( σ 3. σ 3
Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials Brittle materials are materials that display Hookean behavior (linear relationship between stress and strain) and which
More informationMECHANICS OF SOLIDS  BEAMS TUTORIAL 1 STRESSES IN BEAMS DUE TO BENDING. On completion of this tutorial you should be able to do the following.
MECHANICS OF SOLIDS  BEAMS TUTOIAL 1 STESSES IN BEAMS DUE TO BENDING This is the first tutorial on bending of beams designed for anyone wishing to study it at a fairly advanced level. You should judge
More informationTorsion Tests. Subjects of interest
Chapter 10 Torsion Tests Subjects of interest Introduction/Objectives Mechanical properties in torsion Torsional stresses for large plastic strains Type of torsion failures Torsion test vs.tension test
More informationStrip Flatness Prediction in a 4 High Tandem Mill Using a Dynamic Model.
Strip Flatness Prediction in a 4 High Tandem Mill Using a Dynamic Model. M. A. BelloGomez 1, M. P. GuerreroMata 1, L. A. Leduc Lezama 1, T. P. Berber Solano 1, L. Nieves 2, F. Gonzalez 2, H. R. Siller
More informationIMPROVING THE STRUT AND TIE METHOD BY INCLUDING THE CONCRETE SOFTENING EFFECT
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 2, MarchApril 2016, pp. 117 127, Article ID: IJCIET_07_02_009 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=2
More informationESCUELA TÉCNICA SUPERIOR DE INGENIEROS INDUSTRIALES Y DE TELECOMUNICACIÓN
ESCUELA TÉCNICA SUPERIOR DE INGENIEROS INDUSTRIALES Y DE TELECOMUNICACIÓN Titulación: INGENIERO INDUSTRIAL Título del proyecto: MODELING CRACKS WITH ABAQUS Pablo Sanchis Gurpide Pamplona, 22 de Julio del
More informationMechanical Properties
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
More informationINJECTION MOLDING COOLING TIME REDUCTION AND THERMAL STRESS ANALYSIS
INJECTION MOLDING COOLING TIME REDUCTION AND THERMAL STRESS ANALYSIS Tom Kimerling University of Massachusetts, Amherst MIE 605 Finite Element Analysis Spring 2002 ABSTRACT A FEA transient thermal structural
More informationInternational Journal of Engineering ResearchOnline A Peer Reviewed International Journal Articles available online http://www.ijoer.
RESEARCH ARTICLE ISSN: 23217758 DESIGN AND DEVELOPMENT OF A DYNAMOMETER FOR MEASURING THRUST AND TORQUE IN DRILLING APPLICATION SREEJITH C 1,MANU RAJ K R 2 1 PG Scholar, M.Tech Machine Design, Nehru College
More informationSolved with COMSOL Multiphysics 4.3
Vibrating String Introduction In the following example you compute the natural frequencies of a pretensioned string using the 2D Truss interface. This is an example of stress stiffening ; in fact the
More informationFinite Element Formulation for Beams  Handout 2 
Finite Element Formulation for Beams  Handout 2  Dr Fehmi Cirak (fc286@) Completed Version Review of EulerBernoulli Beam Physical beam model midline Beam domain in threedimensions Midline, also called
More informationThe elements used in commercial codes can be classified in two basic categories:
CHAPTER 3 Truss Element 3.1 Introduction The single most important concept in understanding FEA, is the basic understanding of various finite elements that we employ in an analysis. Elements are used for
More informationSolid Mechanics. Stress. What you ll learn: Motivation
Solid Mechanics Stress What you ll learn: What is stress? Why stress is important? What are normal and shear stresses? What is strain? Hooke s law (relationship between stress and strain) Stress strain
More informationApplying the Wheatstone Bridge Circuit
Applying the Wheatstone Bridge Circuit by Karl Hoffmann W15691.0 en Applying the Wheatstone Bridge Circuit by Karl Hoffmann Contents: 1 Introduction...1 2 Elementary circuits with strain gages...5 2.1
More informationUSE OF CFRP LAMINATES FOR STRENGTHENING OF REINFORCED CONCRETE CORBELS
International Journal of Civil Engineering and Technology (IJCIET) Volume 6, Issue 11, Nov 2015, pp. 1120, Article ID: IJCIET_06_11_002 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=6&itype=11
More informationCOMBINED STRESSES IN GUSSET PLATES W. A. Thornton, Ph.D., P.E.* GENERAL
COMBINED STRESSES IN GUSSET PLATES W. A. Thornton, Ph.D., P.E.* GENERAL It has been the traditional approach in the design of connections in the United States, to consider only simple stresses, i.e., shear,
More informationFDM Part Quality Manufactured with Ultem*9085
FDM Part Quality Manufactured with Ultem*9085 A. Bagsik 1,2, V. Schöppner 1, E. Klemp 2 1 Kunststofftechnik Paderborn (KTP),Universität Paderborn, D33102 Paderborn, Germany 2 Direct Manufacturing Research
More informationFatigue. 3. Final fracture (rough zone) 1. Fatigue origin. 2. Beach marks (velvety zone)
Fatigue Term fatigue introduced by Poncelet (France) 1839 progressive fracture is more descriptive 1. Minute crack at critical area of high local stress (geometric stress raiser, flaws, preexisting cracks)
More informationStress and deformation of offshore piles under structural and wave loading
Stress and deformation of offshore piles under structural and wave loading J. A. Eicher, H. Guan, and D. S. Jeng # School of Engineering, Griffith University, Gold Coast Campus, PMB 50 Gold Coast Mail
More informationFinite Element Formulation for Plates  Handout 3 
Finite Element Formulation for Plates  Handout 3  Dr Fehmi Cirak (fc286@) Completed Version Definitions A plate is a three dimensional solid body with one of the plate dimensions much smaller than the
More informationSEISMIC RETROFITTING TECHNIQUE USING CARBON FIBERS FOR REINFORCED CONCRETE BUILDINGS
Fracture Mechanics of Concrete Structures Proceedings FRAMCOS3 AEDIFICA TIO Publishers, D79104 Freiburg, Germany SEISMIC RETROFITTING TECHNIQUE USING CARBON FIBERS FOR REINFORCED CONCRETE BUILDINGS H.
More informationVersion default Titre : SSNP161 Essais biaxiaux de Kupfer Date : 10/10/2012 Page : 1/8 Responsable : François HAMON Clé : V6.03.161 Révision : 9783
Titre : SSNP161 Essais biaxiaux de Kupfer Date : 10/10/2012 Page : 1/8 SSNP161 Biaxial tests of Summarized Kupfer: Kupfer [1] was interested to characterize the performances of the concrete under biaxial
More information4.3 Results... 27 4.3.1 Drained Conditions... 27 4.3.2 Undrained Conditions... 28 4.4 References... 30 4.5 Data Files... 30 5 Undrained Analysis of
Table of Contents 1 One Dimensional Compression of a Finite Layer... 3 1.1 Problem Description... 3 1.1.1 Uniform Mesh... 3 1.1.2 Graded Mesh... 5 1.2 Analytical Solution... 6 1.3 Results... 6 1.3.1 Uniform
More informationFatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY)
Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY) Ali Fatemi, Jonathan Williams and Farzin Montazersadgh Professor and Graduate
More informationNUMERICAL MODELLING OF PIEZOCONE PENETRATION IN CLAY
NUMERICAL MODELLING OF PIEZOCONE PENETRATION IN CLAY Ilaria Giusti University of Pisa ilaria.giusti@for.unipi.it Andrew J. Whittle Massachusetts Institute of Technology ajwhittl@mit.edu Abstract This paper
More informationTensile Testing Laboratory
Tensile Testing Laboratory By Stephan Favilla 0723668 ME 354 AC Date of Lab Report Submission: February 11 th 2010 Date of Lab Exercise: January 28 th 2010 1 Executive Summary Tensile tests are fundamental
More informationStudy of Energy Absorption of Rectangular Tube of Bumper of Light Commercial Vehicle during Oblique Loading
Study of Energy Absorption of Rectangular Tube of Bumper of Light Commercial Vehicle during Oblique Loading S. B. Tuljapure 1, Dr. S. S. Sarawade 2 Ph. D. Student, Department of Mechanical Engineering,
More informationIntroduction to Plates
Chapter Introduction to Plates Plate is a flat surface having considerabl large dimensions as compared to its thickness. Common eamples of plates in civil engineering are. Slab in a building.. Base slab
More informationChapter 2 Laser Diode Beam Propagation Basics
Chapter 2 Laser Diode Beam Propagation Basics Abstract Laser diode beam propagation characteristics, the collimating and focusing behaviors and the M 2 factor are discussed using equations and graphs.
More informationANALYSIS OF A LAP JOINT FRICTION CONNECTION USING HIGH STRENGTH BOLTS
Nordic Steel Construction Conference 212 Hotel Bristol, Oslo, Norway 57 September 212 ANALYSIS OF A LAP JOINT FRICTION CONNECTION USING HIGH STRENGTH BOLTS Marouene Limam a, Christine Heistermann a and
More informationDOING PHYSICS WITH MATLAB COMPUTATIONAL OPTICS RAYLEIGHSOMMERFELD DIFFRACTION INTEGRAL OF THE FIRST KIND
DOING PHYSICS WITH MATLAB COMPUTATIONAL OPTICS RAYLEIGHSOMMERFELD DIFFRACTION INTEGRAL OF THE FIRST KIND THE THREEDIMENSIONAL DISTRIBUTION OF THE RADIANT FLUX DENSITY AT THE FOCUS OF A CONVERGENCE BEAM
More information8.2 Elastic Strain Energy
Section 8. 8. Elastic Strain Energy The strain energy stored in an elastic material upon deformation is calculated below for a number of different geometries and loading conditions. These expressions for
More informationLap Fillet Weld Calculations and FEA Techniques
Lap Fillet Weld Calculations and FEA Techniques By: MS.ME Ahmad A. Abbas Sr. Analysis Engineer Ahmad.Abbas@AdvancedCAE.com www.advancedcae.com Sunday, July 11, 2010 Advanced CAE All contents Copyright
More informationBEHAVIOR OF WELDED TSTUBS SUBJECTED TO TENSILE LOADS
BEHAVIOR OF WELDED TSTUBS SUBJECTED TO TENSILE LOADS R.A. Herrera 1, G. Desjouis 2, G. Gomez 2, M. Sarrazin 3 1 Assistant Professor, Dept. of Civil Engineering, University of Chile, Santiago, Chile 2
More informationNew approaches in Eurocode 3 efficient global structural design
New approaches in Eurocode 3 efficient global structural design Part 1: 3D model based analysis using general beamcolumn FEM Ferenc Papp* and József Szalai ** * Associate Professor, Department of Structural
More informationNonlinear Models of Reinforced and Posttensioned Concrete Beams
111 Nonlinear Models of Reinforced and Posttensioned Concrete Beams ABSTRACT P. Fanning Lecturer, Department of Civil Engineering, University College Dublin Earlsfort Terrace, Dublin 2, Ireland. Email:
More informationChapter 5 Bridge Deck Slabs. Bridge Engineering 1
Chapter 5 Bridge Deck Slabs Bridge Engineering 1 Basic types of bridge decks Insitu reinforced concrete deck (most common type) Precast concrete deck (minimize the use of local labor) Open steel grid
More informationStresses in Beam (Basic Topics)
Chapter 5 Stresses in Beam (Basic Topics) 5.1 Introduction Beam : loads acting transversely to the longitudinal axis the loads create shear forces and bending moments, stresses and strains due to V and
More informationLOAD DEFLECTION DIAGRAM OF OVERREINFORCED CONCRETE BEAMS
Fracture Mechanics of Concrete Structures Proceedings FRAMCOS3 AEDIFICATIO Publishers, D79104 Freiburg, Germany LOAD DEFLECTION DIAGRAM OF OVERREINFORCED CONCRETE BEAMS A. Bascoul Laboratoire Materiaux
More informationMechanical Properties and Fracture Analysis of Glass. David Dutt Chromaglass, Inc.
Mechanical Properties and Fracture Analysis of Glass David Dutt Chromaglass, Inc. IES ALC Williamsburg 2006 2 IES ALC Williamsburg 2006 3 Outline The Ideal The Practical The Reality IES ALC Williamsburg
More informationStress Analysis Verification Manual
Settle3D 3D settlement for foundations Stress Analysis Verification Manual 00701 Rocscience Inc. Table of Contents Settle3D Stress Verification Problems 1 Vertical Stresses underneath Rectangular Footings
More informationEstimation of Adjacent Building Settlement During Drilling of Urban Tunnels
Estimation of Adjacent Building During Drilling of Urban Tunnels Shahram Pourakbar 1, Mohammad Azadi 2, Bujang B. K. Huat 1, Afshin Asadi 1 1 Department of Civil Engineering, University Putra Malaysia
More informationCRITERIA FOR PRELOADED BOLTS
National Aeronautics and Space Administration Lyndon B. Johnson Space Center Houston, Texas 77058 REVISION A JULY 6, 1998 REPLACES BASELINE SPACE SHUTTLE CRITERIA FOR PRELOADED BOLTS CONTENTS 1.0 INTRODUCTION..............................................
More informationDYNAMIC ANALYSIS OF THICK PLATES SUBJECTED TO EARTQUAKE
DYNAMIC ANALYSIS OF THICK PLATES SUBJECTED TO EARTQUAKE ÖZDEMİR Y. I, AYVAZ Y. Posta Adresi: Department of Civil Engineering, Karadeniz Technical University, 68 Trabzon, TURKEY Eposta: yaprakozdemir@hotmail.com
More information3 Concepts of Stress Analysis
3 Concepts of Stress Analysis 3.1 Introduction Here the concepts of stress analysis will be stated in a finite element context. That means that the primary unknown will be the (generalized) displacements.
More informationStructural Axial, Shear and Bending Moments
Structural Axial, Shear and Bending Moments Positive Internal Forces Acting Recall from mechanics of materials that the internal forces P (generic axial), V (shear) and M (moment) represent resultants
More informationIntroduction to Mechanical Behavior of Biological Materials
Introduction to Mechanical Behavior of Biological Materials Ozkaya and Nordin Chapter 7, pages 127151 Chapter 8, pages 173194 Outline Modes of loading Internal forces and moments Stiffness of a structure
More informationMETHODS FOR ACHIEVEMENT UNIFORM STRESSES DISTRIBUTION UNDER THE FOUNDATION
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 2, MarchApril 2016, pp. 4566, Article ID: IJCIET_07_02_004 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=2
More informationOpen Channel Flow Measurement Weirs and Flumes
Open Channel Flow Measurement Weirs and Flumes by Harlan H. Bengtson, PhD, P.E. 1. Introduction Your Course Title Here Measuring the flow rate of water in an open channel typically involves some type of
More informationDESIGN AND ANALYSIS OF BRIDGE WITH TWO ENDS FIXED ON VERTICAL WALL USING FINITE ELEMENT ANALYSIS
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 2, MarchApril 2016, pp. 3444, Article ID: IJCIET_07_02_003 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=2
More informationFatigue Crack Growth in Metals under Pure Mode III: Reality or Fiction?
Fatigue Crack Growth in Metals under Pure Mode III: Reality or Fiction? J. Pokluda 1, R. Pippan 2, K. Slámecka 1 and O. Kolednik 2 1 Institute of Engineering Physics, Brno University of Technology, Technická
More informationCOMPLEX STRESS TUTORIAL 3 COMPLEX STRESS AND STRAIN
COMPLX STRSS TUTORIAL COMPLX STRSS AND STRAIN This tutorial is not part of the decel unit mechanical Principles but covers elements of the following sllabi. o Parts of the ngineering Council eam subject
More informationDUCTILE DAMAGE PARAMETERS IDENTIFICATION FOR NUCLEAR POWER PLANTS EXPERIMENTAL PART. Antonín PRANTL, Jan DŽUGAN, Pavel KONOPÍK
DUCTILE DAMAGE PARAMETERS IDENTIFICATION FOR NUCLEAR POWER PLANTS EXPERIMENTAL PART Antonín PRANTL, Jan DŽUGAN, Pavel KONOPÍK Škoda JS a.s., Pilsen, Czech Republic, EU, antonin.prantl@skodajs.cz COMTES
More informationShell Elements in ABAQUS/Explicit
ABAQUS/Explicit: Advanced Topics Appendix 2 Shell Elements in ABAQUS/Explicit ABAQUS/Explicit: Advanced Topics A2.2 Overview ABAQUS/Explicit: Advanced Topics ABAQUS/Explicit: Advanced Topics A2.4 Triangular
More informationMECHANICS OF SOLIDS  BEAMS TUTORIAL 2 SHEAR FORCE AND BENDING MOMENTS IN BEAMS
MECHANICS OF SOLIDS  BEAMS TUTORIAL 2 SHEAR FORCE AND BENDING MOMENTS IN BEAMS This is the second tutorial on bending of beams. You should judge your progress by completing the self assessment exercises.
More informationInvestigation of Stress Intensity Factor of Axial Compressor Blade of Helicopter
Investigation of Stress Intensity Factor of Axial Compressor Blade of Helicopter Neelesh V K Mr. Manjunath M V Mr. Devaraj Dept. of Mechanical Engineering Asst prof, Dept. of Mechanical Engineering Asst
More informationLaser cutting of thick ceramic substrates by controlled fracture technique
Journal of Materials Processing Technology 136 (2003) 166 173 Laser cutting of thick ceramic substrates by controlled fracture technique ChwanHuei Tsai *, HongWen Chen Institute of Mechatronic Engineering,
More informationFracture and strain rate behavior of airplane fuselage materials under blast loading
EPJ Web of Conferences 6, 6 42017 (2010) DOI:10.1051/epjconf/20100642017 Owned by the authors, published by EDP Sciences, 2010 Fracture and strain rate behavior of airplane fuselage materials under blast
More informationDEVELOPMENT OF A NEW TEST FOR DETERMINATION OF TENSILE STRENGTH OF CONCRETE BLOCKS
1 th Canadian Masonry Symposium Vancouver, British Columbia, June 5, 013 DEVELOPMENT OF A NEW TEST FOR DETERMINATION OF TENSILE STRENGTH OF CONCRETE BLOCKS Vladimir G. Haach 1, Graça Vasconcelos and Paulo
More informationA quadrilateral 2D finite element based on mixed interpolation of tensorial
A quadrilateral 2D finite element based on mixed interpolation of tensorial components Eduardo N. Dvorkin and Sara I. Vassolo* Instituto de Materiales y Estructuras, Facultad de Ingenieria, Universidad
More information